Evolution of structural, mechanical and tribological properties of Ni
MWCNT coatings as a function of annealing temperature
, Mauro Callistia
, Alberto Mirandab
, Brian McKayb
, Ioanna Deligkiozic
Tatjana Kosanovic Milickovicd
, Alexandros Zoikis-Karathanasisd
, Kostas Hrissagisd
, Tomas Polcara
aNational Centre for Advanced Tribology at Southampton, Faculty of Engineering and the Environment, University of Southampton, Southampton SO17 1BJ, UK bInstitute of Materials and Manufacturing, Brunel University, London UB8 3PH, UK
Centre for Technology Research and Innovation, Limassol 3106, Cyprus
Centre for Research and Technology Hellas (CERTH/IRETETH), Trikala GR42100, Greece
Dip. Chimica, Materiali e Ing. Chimica Giulio Natta, Politecnico di Milano, Milano 20131, Italy
a b s t r a c t
a r t i c l e i n f o
Article history: Received 7 April 2016 Revised 30 May 2016
Accepted in revised form 5 June 2016 Available online 06 June 2016
The structural, mechanical and tribological properties of Ni–P/MWCNT coatings annealed at various tempera-tures (350–500 °C) were investigated using XRD, SEM, nanoindentation and tribometer to determine the optimal annealing temperature for their enhanced tribological properties. The results showed that the annealed coatings comprised a hard Ni3P phase, and consequently presented a higher hardness (from 7.0 ± 0.3 to 8.2 ± 1.4 GPa)
than the as-plated sample (6.0 ± 0.9 GPa). With the annealing temperature increasing from 350 °C to 500 °C, the crystallinity of coating was enhanced with larger crystal grains of Ni and Ni3P, which led to a decline in
hard-ness (from 8.2 to 7.0 GPa) due to the Hall-Petch effect. Owing to the lubrication effect of H3PO4arising from the
tribochemical reaction of Ni3P with ambient environment, the annealed samples exhibited lower friction
coefﬁ-cients (0.71 ~ 0.86) compared to the as-plated coating (0.87). A combination of low surface roughness and the reduction of oxides on wear track contributed to the lowest friction coefﬁcient of Ni–P/MWCNT annealed at 400 °C. However, the decomposition of amorphous carbon in MWCNT over 380 °C produced less dense coatings (for annealing temperatures 400–500 °C), and their incompact structure led to a higher wear rate (2.9– 3.0 × 10−5mm3/Nm) compared to the as-plated sample (2.4 × 10−5mm3/Nm). In contrast, Ni
–P/MWCNT coat-ing annealed at 350 °C (b380 °C) exhibited a better wear resistance (4.3 × 10−6mm3/Nm). Thus, 350 °C was
found to be the optimal annealing temperature to lower the friction coefﬁcient and enhance the wear resistance of Ni–P/MWCNT coatings.
© 2016 Elsevier B.V. All rights reserved.
Keywords: Nickel-phosphorus MWCNT Electrodeposition Tribology Annealing 1. Introduction
Owing to their excellent resistance to both wear and corrosion, electroplated hard chrome coatings are one of the widely used surface treatments in the aerospace, automotive and shipping industries[1– 3]. Nevertheless, with a growing awareness on environment protection and human health, researchers are looking for viable alternative to hard chrome coatings to avoid the hazardous Cr6+(a genotoxic carcinogen) in electrolytic baths[4–7].
In order to minimise additional costs for plating industry, re-searchers have concentrated their attention on Ni–P coatings using existing equipment. Consequently, several studies investigated the in-ﬂuence of pH value, surfactant, bath parametersand post-treatment[11,12]in order to optimise the structural and tribological
properties of Ni–P coatings. Nevertheless, the low hardness of the as-plated Ni–P coatings (400–500 HV0.025) still stands in its way of a wide application in tribologyﬁeld, where hardness is deemed as a vital property. Therefore, various reinforcing particles have been intro-duced into Ni–P coatings to increase their hardness and as a conse-quence enhance their tribological properties.
Amongst SiC, TiN, TiO2, SiO2[16,17], WC, Al2O3
, B4Cand CNT[21–23]reinforcing particles, SiC and MWCNT
in-corporations demonstrated a greater enhancement in hardness (ΔH N 260 HV0.01). Compared with SiC, CNT has shown an extremely high Young's modulus up to 1.0 TPa and a high tensile strength around 60 GPa. Moreover, CNT is expected to provide superior lubrication effect than SiC due to its integrated molecule, in which the carbon atoms are bonded with sp2hybrid. For instance, Chen et al.found that
Ni/CNT composite coatings exhibited a lower friction coefﬁcient (0.075) than Ni/SiC coatings (0.130). Tu et al.[26,27]pointed out that MWCNT co-deposition reduced the friction coefﬁcient of Ni–P coatings down to
⁎ Corresponding author.
E-mail addresses:email@example.com,firstname.lastname@example.org(Q. Wang).
0257-8972/© 2016 Elsevier B.V. All rights reserved.
Contents lists available atScienceDirect
Surface & Coatings Technology
0.063 compared to 0.124 for SiC reinforced ones. A similar result was also reported in Ref.as listed inTable 1. However, in current litera-ture, only a few studies have focused on the role of heat treatment in de-termining the tribological properties of Ni–P/MWCNT coatings[23,25, 27,29,30]. More importantly, the coatings in the above studies were all deposited using electroless technique, whilst the chosen interval of an-nealing temperature was too large (200 °C) to help us understand the tendencies from 200 to 400 °C and from 400 to 600 °C. Thus, it is of par-amount importance to study the detailed evolution of the tribological properties for annealed Ni–P/MWCNT coatings with a small interval of temperature, especially for the coatings fabricated by using electrodeposition.
In this present study, electrodeposited Ni–P/MWCNT coatings annealed at four different temperatures (350, 400, 450 and 500 °C) as well as the as-plated coating (50 °C) were compared in order to study the effect of heat treatment on their tribological properties. The correla-tion between annealing temperature, microstructure, mechanical and tribological properties of Ni–P/MWCNT coatings was subsequently elucidated.
2. Experimental details
2.1. Composite coatings electroplating and annealing
Multi-walled carbon nanotubes (MWCNTs) with 3–15 walls (Inner diameter 2–6 nm and outer diameter 5–20 nm) and length of 1– 10μm were selected as reinforcing particles (supplied by EMFUTUR Technologies). In order to evaluate the quality of MWCNTs, a Renishaw inVia confocal Raman microscope with an excitation energy of 2.54 eV and a Raman shift from 800 to 2000 cm−1was used. In addition, a si-multaneous thermogravimetric analysis (TGA) and differential scan-ning calorimetry (DSC) analysis at a heating rate of 10 °C/min was conducted in a He atmosphere (40 mL/min) to assess the thermal stabil-ity of MWCNTs up to 900 °C (NETZCH STA 409 PC Luxx). After being dis-persed in 10 ml of ethanol in an ultrasonic bath for 2 min, two drops of the MWCNTs suspension were pipetted onto a 400 # Cu grid, and then naturally dried under ambient condition prior to the observation by using transmission electron microscope (TEM) operated at 80 kV (JEOL 2100 FEG). To remove surface contaminants on the substrates, the carbon steel plates with dimensions of 4 × 6 cm2were anodized
in NaOH (1.25 M) and immersed in HCl (1:8) consecutively. Afterwards, they were covered by galvanic tape (3 M 470 Electroplating and Anod-izing Vinyl Tape) leaving an exposed area of 4 × 4 cm2. Suzuki et al.
and Li et al.found that the Ni–P/MWCNT composite coatings with a lower concentration of CNT (0.7% mass) exhibited superior tribological properties. Thus, 1 g/L of MWCNT was loaded into the electrolytic bath in this study to keep a low concentration of MWCNT in Ni–P/MWCNT coatings. The plating electrolyte contained nickel sulphate as nickel source, phosphorous acid as P source and nickel chloride to support the dissolution of Ni–S anode. Based on the hardness and surface rough-ness (Ra) of Ni–P/MWCNT coatings as a function of current density (5,
10, 15 and 20 A dm−2) in our previous work, Ni–P/MWCNT coating (4.9 w.t% P and 60μm thick) electroplated at 20 A dm−2is chosen as
the subject in this paper. In order to ensure a uniform electrolyte solu-tion, a magnetic stirring at 300 rpm was applied during the entire electroplating process. The deposition parameters for the preparation of the composite coatings are listed inTable 2.
Using an electric furnace, the as-plated Ni–P/MWCNT coatings (50 ° C) were annealed at 350, 400, 450 and 500 °C, and hereafter denoted as Ni–P/MWCNT-50, Ni–P/MWCNT-350, Ni–P/MWCNT-400, Ni–P/ MWCNT-450 and Ni–P/MWCNT-500. During heat treatment, a constant heating rate of 5 °C/min was maintained until the target temperature was reached. After a holding time of 1 h, samples were cooled naturally to room temperature. In order to remove the surface oxides by heat treatment, all of the specimens were mechanically polished using 0.3μm Al2O3suspension for 5 min.
2.2. Microstructure and mechanical properties of composite coatings The morphology of the Ni–P/MWCNT coatings after mechanical polishing was observed by scanning electron microscope (SEM) (JEOL-JSM-6500F), and their chemical composition was analyzed by energy dispersive spectroscopy (EDS) equipped on SEM (FEI Quanta 200). By using X-ray diffraction (XRD) with a Cu-Kαradiation (Siemens
D-5000), the phase conditions of the as-plated and annealed coatings were characterized within a 2θ range from 20° to 100° at a scanning rate of 5°/min and a step size of 0.05°. To investigate the mechanical properties of the Ni–P/MWCNT coatings, nanoindentation (Micromaterials) under a penetration depth of 500 nm (b10% of the coatings thickness) was carried out. In order to ensure the reliability of data, 10 nanoindentations were conducted for each coating. The sur-face roughness (Ra) of coatings after polishing was measured using a 3D optical microscope (Inﬁnite Focus).
2.3. Evaluation of tribological properties
The friction and wear behavior of Ni–P/MWCNT coatings under am-bient condition was evaluated by using a reciprocating tribometer (TE77, Phoenix Tribology, Ltd.). Since the potential application of Ni– P/MWCNT coatings on crankshaft, 52,100 steel balls (Ø 6 mm), as a common material for linkage, was selected as counterpart in this study. In order to achieve the friction coefﬁcient within the steady peri-od, which appears after running-in period and before the failure of coat-ings, the stroke length, frequency and applied load of the tribotest were kept at 10 mm, 5 Hz and 10 N respectively for a duration of 1 h. All of the tribotests were repeated twice to ensure the reliability of data, with a third test necessary if the relative error of friction coefﬁcient was over
Mechanical and tribological properties of Ni and Ni–P coatings alloying with SiC and CNT particles.
Reference Coatings Particles Hardness Friction coefﬁcient Wear depth or mass loss Chen et al. Ni SiC 725 HV0.025 0.130 11.2μm
CNT 865 HV0.025 0.075 6.6μm
Tu et al.[26,27] Ni–P SiC 550 HV0.05 0.124 8.5 mg
MWCNT 520 HV0.05 0.063 6.2 mg
Chen et al. Ni–P SiC 725 HV0.025 0.147 5.7 mg MWCNT 946 HV0.025 0.122 3.0 mg
Electro-deposition conditions of Ni–P/MWCNT coatings. Temperature 50 ± 2 °C
pH 1 ± 0.2
MWCNT load 1 g/L Current density 20 Adm−2 Substrate Steel platelet
5%. A 3D optical microscope (Inﬁnite Focus) was subsequently used to analyze the contours of wear tracks. Accordingly, the wear volume of coatings can be determined from the product of cross-section area (A) and wear length (L). In addition, the morphology of wear tracks were observed by SEM (JEOL-JSM-6500F), and their corresponding chemical compositions were analyzed using EDS (Inca Energy 350).
3. Results and discussions
3.1. Characterization of MWCNT and Ni–P/MWCNT composite coatings The TEM images of MWCNT under different magniﬁcations are shown inFig. 1a and b. It is clear that the MWCNTs used in this study are of various diameters as stated in experimental details. The XRD
spectrum of MWCNT inFig. 1c demonstrates its common crystallinity whilst the Raman spectrum inFig. 1d indicates the presence of amor-phous carbon (a-C). Consequently, as seen inFig. 2, two endother-mic peaks around 420 °C and 500 °C in DSC trace are closely associated with the decomposition of a-C. As a result, a sharp weight loss is ob-served in TGA diagram from 380 °C to 500 °C. It is in contrast to pure MWCNT (i.e. without any amorphous carbon), which should remain stable up to 2800 °C.
As seen inFig. 3a, the XRD spectrum of the Ni–P/MWCNT-50 coating exhibits two broad peaks at 44.5° and 97.8°, which are related to Ni (111) and Ni (222) (JCPDS 00-004-0850). Howev-er, the crystallinity of Ni is signiﬁcantly enhanced after anneal-ing, and continues to increase with increasing annealing temperature. In addition, new diffraction peaks (around 42.8°, 43.6°, 60.2°, 74.9° and etc.) are observed in XRD spectra after heat treatment, which were identiﬁed as Ni3P crystal (JCPDS
01–089-2743) by DIFFRAC.EVA software (Siemens Energy and Automatization, Inc.). The size evolution of Ni (111) and Ni3P
(231) grains as a function of annealing temperature was calcu-lated according to the Scherrer's equation , and the results are presented in Fig. 3b. It is obvious that the crystal grains of Ni (111) and Ni3P (231) grow from 6 nm to 50 nm and
from 34 nm to 59 nm, respectively, as the annealing tempera-ture increases. Note that no MWCNT was detected in diffractograms of Ni–P/MWCNT coatings because of a very low incorporation amount (1.9 wt.%).
The surface morphology and individual roughness (Ra) of the Ni–P/MWCNT coatings after polishing are shown in Fig. 4. The Ni–P/MWCNT-50 coating exhibits the highest Ra of 7.9 ± 0.5 μm with obvious agglomeration structure. In contrast, few agglomeration structures are evident in the annealed coatings and the Ni–P/MWCNT-400 coating exhibits the lowest Ra of 6.7 ± 0.2 μm. This lower asperity has a beneﬁcial effect on its friction behavior, which will be discussed elsewhere (in Section 3.3).
Fig. 1. (a) (b) TEM images (c) XRD and (d) Raman spectra of MWCNT.
Fig. 2. Differential scanning calorimetry (DSC) and thermogravimetric analysis (TGA) of MWCNT under a He atmosphere.
3.2. Characterization of mechanical properties
The hardness (H) and reduced elastic modulus (Er) of each coating
were obtained from loading-unloading curves by applying the Oliver and Pharr method, whilst the recovery of elasticity (Re) was
calcu-lated via maximum (hmax) and residual (hf) depths. As listed inTable 3,
all of the annealed specimens exhibit a higher hardness (7.0 ± 0.3– 8.2 ± 1.4 GPa) than the as-plated one (6.0 ± 0.9 GPa) due to the forma-tion of a hard intermetallic Ni3P crystalline phase. Nevertheless, the
increasing grain size of Ni (111) and Ni3P (231) with increasing
temper-ature leads to a reduction in hardness from 8.2 to 7.0 GPa based on the Hall-Petch effect. Since elastic modulus has an equal role as hardness in determining tribological properties, some researchers have suggested using the ratios of H/Erand H3/Er2for tribology prediction, as they are
proportional to the resistance to elastic strain and plastic deformation, respectively. Moreover, coatings with a superior Reshould
encoun-ter lower plastic deformation. Thus, according to the values inTable 3, the Ni–P/MWCNT-350 coating is expected to present the best tribolog-ical performance due to a combination of the highest H/Er, H3/Er2and Re,
followed by the Ni–P/MWCNT-400 coating.
3.3. Evaluation of friction
Fig. 5shows the friction behavior of Ni–P/MWCNT coatings as a function of sliding time. It is clear that the friction coefﬁcient of all the samples decreases gradually from its original value to a steady state value after a speciﬁc ‘running-in’ period. Due to a relatively rougher sur-face with a higher Ra (Fig. 4a&b), the Ni–P/MWCNT-50 and Ni–P/ MWCNT-350 coatings encounter a longer‘running-in’ period - more time is needed to remove large asperities. In contrast, the Ni–P/ MWCNT-450 and Ni–P/MWCNT-500 coatings exhibit a shorter ‘run-ning-in’ period due to a lower Ra (Fig. 4d&e). Interestingly, the Ni–P/ MWCNT-400 coating presents the longest‘running-in’ period (around 2100 s) even with the smoothest morphology. In principle, surface qual-ity largely determines the length of the‘running-in’ period, but hard-ness is another important factor that needs to be considered. As listed inTable 3, the Ni–P/MWCNT-400 coating exhibits the highest hardness (8.2 GPa), which contributes to a low rate of asperity removal. As a re-sult, the friction coefﬁcient of Ni–P/MWCNT-400 coating takes more time to reach a steady state; a similar phenomenon was reported in Ref.. Furthermore, it is worth noting that the smoothest morpholo-gy of the Ni–P/MWCNT-400 coating contributes to a steady friction be-havior during the entire tribotest. In contrast, dramaticﬂuctuations of
Fig. 3. (a) XRD spectra and (b) crystalline sizes of Ni (111) and Ni3P (231) of Ni–P/MWCNT coatings annealed at different temperatures.
the friction coefﬁcient are observed on the friction behavior of the other coatings.
By averaging the friction coefﬁcient attained during steady state, the mean-steady friction coefﬁcient of each coating is illustrated inFig. 6a. Obviously, all of the annealed coatings exhibit a lower friction coef ﬁ-cient (0.71 ± 0.031 ~ 0.86 ± 0.042) than the as-plated condition (0.87 ± 0.055). This discrepancy is attributed to the different tribochemical reactions during the tribotest as described below:
4Niþ 3O2¼ 2Ni2O3 ΔG298 f ¼ −287:6kJ mol−1 ð1Þ 2Ni3Pþ 7O2¼ 3Ni2O3þ P2O5 ΔG298 f ¼ −1364:7kJ mol−1 ð2Þ P2O5þ 3H2O¼ 2H3PO4 ΔG298 f ¼ −144:1kJ mol−1 ð3Þ
According to the standard Gibbs free energy[41–43], tribochemical reactions (1–3) can occur spontaneously. Incongruent with the tribochemical reaction of the Ni–P/MWCNT-50 coating (Eq.(1)), the ox-idation of Ni3P in annealed coatings (Eqs.(2) and (3)) generates not
only Ni2O3but also P2O5, which is extremely unstable in air.
Subse-quently, the generated P2O5absorbs the moisture from its ambient
en-vironment to form orthophosphoric acid (H3PO4). It has been reported
that, in H3PO4environment, a lubricant gel containing Fe-P-O and
elec-trical double layer effect contributed to a drop in friction coefﬁcient. Hence, all the annealed samples exhibit a lower friction coefﬁcient than the as-plated coating in this study.
It is worth noting that the Ni–P/MWCNT-400 coating exhibits the lowest friction coefﬁcient of 0.71 ± 0.031 amongst the annealed sam-ples. Except for the lubrication effect of H3PO4as mentioned above,
there are two reasons contributing to such a outcome. One is the smoothest morphology (Ra = 6.7 ± 0.2μm), which offers an even con-tact interface between coatings and balls at the beginning stage of tribotest. This favorable condition has a lasting effect during the whole friction behavior, because a lower Ra helps obtain a lower mean-steady friction coefﬁcient[44–46]. The other reason is the amount of oxides formed during the tribotest. In principle, the formation of oxides should decrease friction coefﬁcient due to their softness under dry friction con-dition. However, the adhesion and accumulation of oxides could in-crease the roughness of wear track, thus leading to a higher friction coefﬁcient due to mechanical interlock. As seen inFig. 7, EDS analyses indicate that the wear track on the Ni–P/MWCNT-400 coating contains the lowest concentration of oxygen (3.6 wt.%). Therefore, a lower amount of oxides (Ni2O3and FeOx) was generated in the wear track
resulting in a relatively smoother sliding interface, which contributed to a lower friction.
3.4. Evaluation of wear
Analyzing the coatings wear rate inFig. 6b and the hardness inTable 3, it is found that the wear resistance of Ni–P/MWCNT coatings is not proportional to their hardness. For instance, the coatings annealed at 400, 450 and 500 °C are harder but present higher wear rates (2.9– 3.0 × 10−5mm3/Nm) than the as-plated condition (2.4 × 10−5mm3/
Nm). Furthermore, even with the same hardness (8.2 GPa), the Ni–P/ MWCNT-350 and Ni–P/MWCNT-400 coatings exhibit a big difference in wear rate with one order of magnitude (4.3 × 10−6mm3/Nm and
2.9 × 10−5mm3/Nm). These results imply that there is another key
fac-tor determining their wear resistance.
According to the TGA and DSC shown inFig. 2, the decomposition of amorphous carbon in MWCNTs takes place around 380 °C. Hence, dur-ing the heat treatment, Ni–P/MWCNT-400, Ni–P/MWCNT-450 and Ni– P/MWCNT-500 coatings suffered the decomposition of amorphous car-bon, which deteriorated their compact structure. In contrast, only a lim-ited decomposition of amorphous carbon occurred during the annealing at 350 °C, i.e. the Ni–P/MWCNT-350 coating was still compact and dense after annealing. Therefore, the decomposition of amorphous carbon in MWCNT is the key factor signiﬁcantly limiting the wear resistance of Ni–P/MWCNT coatings. Consequently, Ni–P/MWCNT-400, Ni–P/ MWCNT-450 and Ni–P/MWCNT-500 coatings exhibit a higher wear rate than the softer Ni–P/MWCNT-50 coating, whilst Ni–P/MWCNT-350 coating exhibits the lowest value (4.3 × 10−6mm3/Nm).
Ni–P/MWCNT composite coatings were electroplated on carbon steel plates followed by annealing at various temperatures (350–500 ° C). The evolution of their microstructure, mechanical and tribological properties as a function of annealing temperature was investigated. Conclusions are drawn as follows:
(1) With increasing annealing temperature, the crystallinity of Ni in the Ni–P/MWCNT coatings increased, and a Ni3P phase was
(2) Owing to the presence of the hard Ni3P phase, annealed samples
exhibited a higher hardness (7.0–8.2 GPa) than the as-plated sample (6.0 GPa). However, the increasing grain size led to a drop in hardness from 8.2 GPa to 7.0 GPa due to the Hall-Petch effect.
(3) The Ni–P/MWCNT-400 coating exhibited the lowest friction co-efﬁcient of 0.71 ± 0.03 due to a combination of the lubricious ef-fect of H3PO4from tribochemical reaction, a smoother original
contact surface and fewer oxides formed on the wear track. (4) The decomposition of amorphous carbon in MWCNTs (TN 380 °
C), rather than the hardness, was the key factor to the wear
Mechanical properties of Ni–P/MWCNT coatings at different annealing temperatures. Coatings H (GPa) Er(GPa) H/Er H3/Er2(GPa) Re(%)
Ni–P/MWCNT-50 6.0 ± 0.9 156 ± 6 0.038 0.009 14.7 ± 1.8 Ni–P/MWCNT-350 8.2 ± 1.4 190 ± 14 0.043 0.015 16.6 ± 1.9 Ni–P/MWCNT-400 8.2 ± 0.6 209 ± 7 0.039 0.013 15.2 ± 0.9 Ni–P/MWCNT-450 7.4 ± 0.3 224 ± 14 0.033 0.008 12.8 ± 1.0 Ni–P/MWCNT-500 7.0 ± 0.3 213 ± 4 0.033 0.008 12.6 ± 0.6
Fig. 5. Friction behavior of Ni–P/MWCNT coatings annealed at different temperatures sliding against 52,100 balls.
resistance of Ni–P/MWCNT coatings. Thus, the Ni–P/MWCNT coatings annealed at 400, 450 and 500 °C exhibited a poor wear resistance (wear rate: 2.9–3.0 × 10−5mm3/Nm) while the Ni–
P/MWCNT coating annealed at 350 °C presented the strongest wear resistance (wear rate: 4.3 × 10−6mm3/Nm).
This work has been supported by the collaborative research project Hardalt (Grant No. 606110) funded by the EU's seventh framework programme.
 V.S. Protsenko, F.I. Danilov, V.O. Gordiienko, S.C. Kwon, M. Kim, J.Y. Lee, Electrodeposition of hard nanocrystalline chrome from aqueous sulfate trivalent chromium bath, Thin Solid Films 520 (2011) 380–383.
 K. Ranjbar, M. Sababi, Failure assessment of the hard chrome coated rotors in the downhole drilling motors, Eng. Fail. Anal. 20 (2012) 147–155.
 M. Srivastava, C. Anandan, V.K.W. Grips, Ni–Mo–Co ternary alloy as a replacement for hard chrome, Appl. Surf. Sci. 285 (2013) 167–174.
 Risk & Policy Analysts Limited, Environmental Risk Reduction Strategy and Analysis of Advantages and Drawbacks for Hexavalent Chromium(Norfolk) 2005.
 B. Sonntag, V. Sundaram, Substitution of Cr (VI)-containing coatings by the European automobile industry, Indian Surf. Finish. 1 (2004) 15–26.
 M.D. Cohen, M. Costa, Chromium, in: M. Lippmann (Ed.), Environmental Toxicants: Human Exposures and Their Health Effects, second ed.Wiley, New York 2000, pp. 173–191.
 U.S. Department of Health and Human Services, Agency for Toxic Substances and Disease Registry, Toxicological Proﬁle for Chromium(Atlanta, Georgia) 2012.
 X.W. Zhou, H.M. Jin, L.N. Zhang, Inﬂuence of pH value on microstructure and ther-mal stability of Ni–P electroless coating prepared in acidic condition, Chin. Chem. Lett. 20 (2009) 845–848.
 R. Elansezhian, B. Ramamoorthy, P.K. Nair, Effect of surfactants on the mechanical properties of electroless (Ni–P) coating, Surf. Coat. Technol. 203 (2008) 709–712.
 B. Panja, P. Sahoo, Wear behavior of electroless Ni–P coatings in brine solution and optimization of coating parameters, Procedia Technol. 14 (2014) 173–180.
 M. Novak, D. Vojtech, P. Novak, T. Vitu, Tribological properties of heat-treated elec-troless Ni–P coatings on AZ91 alloy, Appl. Surf. Sci. 257 (2011) 9982–9985.
 J.D. Lin, C.L. Kuo, Effects of hydrogen plasma treatment on microstructure evolution and electrical conductivity of electroless Ni–P coatings on polyimide and glass sub-strates, Surf. Coat. Technol. 209 (2012) 80–89.
Fig. 7. Morphology, contours and the corresponding EDS analyses of wear tracks on Ni–P/MWCNT coatings annealed at different temperatures. Fig. 6. (a) Mean-steady friction coefﬁcient and (b) wear rate of Ni–P/MWCNT coatings annealed at different temperatures.
S.S. Zhang, K.J. Han, L. Cheng, The effect of SiC particles added in electroless Ni–P plating solution on the properties of composite coatings, Surf. Coat. Technol. 202 (2008) 2807–2812.
 I.R. Maﬁ, C. Dehghanian, Studying the effects of the addition of TiN nanoparticles to Ni–P electroless coatings, Appl. Surf. Sci. 258 (2011) 1876–1880.
 S.M.A. Shibli, V.S. Dilimon, Effect of phosphorous content and TiO2-reinforcement on
Ni–P electroless plates for hydrogen evolution reaction, Int. J. Hydrog. Energy 32 (2007) 1694–1700.
Y. Hazan, D. Zimmermann, M. Zgraggen, S. Roos, C. Aneziris, H. Bollier, P. Fehr, T. Graule, Homogeneous electroless Ni–P/SiO2nanocomposite coatings with improved
wear resistance and modiﬁed wear behaviour, Surf. Coat. Technol. 204 (2010) 3464–3470.
 M. Islam, M.R. Azhar, N. Fredj, T.D. Burleigh, O.R. Oloyede, A.A. Almajid, S.I. Shah, In-ﬂuence of SiO2nanoparticles on hardness and corrosion resistance of electroless Ni–
P coatings, Surf. Coat. Technol. 261 (2015) 141–148.
 Z.A. Hamid, S.A.E. Badry, A.A. Aal, Electroless deposition and characterization of Ni– P–WC composite alloys, Surf. Coat. Technol. 201 (2007) 5948–5953.
 S. Karthikeyan, B. Ramamoorthy, Effect of reducing agent and nano Al2O3particles
on the properties of electroless Ni–P coating, Appl. Surf. Sci. 307 (2014) 654–660.
 M.E. Hosseinabadi, K.A. Dorcheh, S.M.M. Vagheﬁ, Wear behavior of electroless Ni–P– B4C composite coatings, Wear 260 (2006) 123–127.
 A. Zarebidaki, S.R. Allahkaram, Effect of surfactant on the fabrication and character-ization of Ni–P–CNT composite coatings, J. Alloys Compd. 509 (2011) 1836–1840.
 M. Alishahi, S.M. Monirvagheﬁ, A. Saatchi, S.M. Hosseini, The effect of carbon nano-tubes on the corrosion and tribological behavior of electroless Ni–P–CNT composite coating, Appl. Surf. Sci. 258 (2012) 2439–2446.
 Z. Yang, H. Xu, Y.L. Shi, M.K. Li, Y. Huang, H.L. Li, The fabrication and corrosion behav-ior of electroless Ni–P-carbon nanotube composite coatings, Mater. Res. Bull. 40 (2005) 1001–1009.
 R. Sudhakar, V.T. Venkatesha, Electrodeposition of Zn–Ni multiwalled carbon nano-tube nanocomposites and their properties, Ind. Eng. Chem. Res. 52 (2013) 6422–6429.
 X.H. Chen, C.S. Chen, H.N. Xiao, H.B. Liu, L.P. Zhou, S.L. Li, G. Zhang, Dry friction and wear characteristics of nickel/carbon nanotube electroless composite deposits, Tribol. Int. 39 (2006) 22–28.
 W.X. Chen, J.P. Tu, Z.D. Xu, W.L. Chen, X.B. Zhang, D.H. Cheng, Tribological properties of Ni–P-multi-walled carbon nanotubes electroless composite coating, Mater. Lett. 57 (2003) 1256–1260.
 W.X. Chen, J.P. Tu, H.Y. Gan, Z.D. Xu, Q.G. Wang, J.Y. Lee, Z.L. Liu, X.B. Zhang, Electro-less preparation and tribological properties of Ni–P-carbon nanotube composite coatings under lubricated condition, Surf. Coat. Technol. 160 (2002) 68–73.
C.S. Chen, X.H. Chen, Z. Yang, W.H. Li, L.S. Xu, B. Yi, Effect of multi-walled carbon nanotubes as reinforcedﬁbres on tribological behaviour of Ni–P electroless coatings, Diam. Relat. Mater. 15 (2006) 151–156.
 W.X. Chen, J.P. Tu, L.Y. Wang, H.Y. Gan, Z.D. Xu, X.B. Zhang, Tribological application of carbon nanotubes in a metal-based composite coating and composites, Carbon 41 (2003) 215–222.
 Q. Shi, W.C. Sun, J. Gao, Y. Wang, M.M. Tian, Effects of heat treatment on mechanical properties of Ni–P–CNT composite coating, Mater. Sci. Forum 817 (1) (2015) 1662–9752.
 Y. Suzuki, S. Arai, M. Endob, Electrodeposition of Ni–P alloy-multiwalled carbon nanotube compositeﬁlms, J. Electrochem. Soc. 157 (2010) D50–D53.
 Z.H. Li, X.Q. Wang, M. Wang, F.F. Wang, H.L. Ge, Preparation and tribological proper-ties of the carbon nanotubes-Ni–P composite coating, Tribol. Int. 39 (2006) 953–957.
 R.A. DiLeo, B.J. Landi, R.P. Raffaelle, Purity assessment of multiwalled carbon nano-tubes by Raman spectroscopy, J. Appl. Phys. 101 (2007) 064307 (1–5).
 P.G. Collins, P. Avouris, Nanotubes for electronics, Sci. Am. 283 (2000) 62–69.
 P. Scherrer, N.G.W. Gottingen, Math-Pys. Kl. 2 (1918) 96–100.
 W.C. Oliver, G.M. Pharr, An improved technique for determining hardness and elas-tic modulus using load and displacement sensing indentation experiments, J. Mater. Res. 7 (1992) 1564–1583.
 D. Nava, C.E. Dávalos, A. Martínez-Hernández, F. Manríquez, Y. Meas, R. Ortega-Borges, J.J. Pérez-Bueno, G. Trejo, Effects of heat treatment on the tribological and corrosion properties of electrodeposited Ni–P alloys, Int. J. Electrochem. Sci. 8 (2013) 2670–2681.
 N.A. Sakharova, J.V. Fernandes, M.C. Oliveira, J.M. Antunes, Inﬂuence of ductile inter-layers on mechanical behaviour of hard coatings under depth-sensing indentation: a numerical study on TiAlN, J. Mater. Sci. 45 (2010) 3812–3823.
 Q.Z. Wang, F. Zhou, X.D. Ding, Z.F. Zhou, C.D. Wang, W.J. Zhang, L.K.-Y. Li, S.-T. Lee, Microstructure and water-lubricated friction and wear properties of CrN(C) coatings with different carbon contents, Appl. Surf. Sci. 268 (2013) 579–587.
Q.Z. Wang, M. Callisti, J. Greer, B. McKay, T.K. Milickovic, A. Zoikis-Karathanasis, I. Deligkiozi, T. Polcar, Effect of annealing temperature on microstructure, mechanical and tribological properties of nano-SiC reinforced Ni–P coatings, Wear 356-357 (2016) 86–93.
 H.G. Zhu, Y.L. Ai, J.L. Li, J. Min, D. Chu, J. Zhao, J. Chen, In situ fabrication ofα-Al2O3
and Ni2Al3reinforced aluminum matrix composites in an Al–Ni2O3system, Adv.
Powder Technol. 22 (2011) 629–633.
 M.H. Sandstrom, D. Bostrom, Determination of standard Gibbs free energy of forma-tion for CaKPO4, CaK4(PO4)2, CaK2P2O7, and Ca10K(PO4)7from solid-state e.m.f.
measurements using yttria stabilised zirconia as solid electrolyte, J. Chem. Thermodyn. 40 (2008) 40–46.
Thermodynamic Properties, in: J.A. Dean (Ed.), Lange's Handbook of Chemistry, Fifteenth ed.Mcgraw-hill, Inc., New York 1998, pp. 545–702.
 R.G. Lu, H.D. Zhang, Y. Mitsuya, K. Fukuzawa, S. Itoh, Inﬂuence of surface roughness and coating on the friction properties of nanometer-thick liquid lubricantﬁlms, Wear 319 (2014) 56–61.
 M.L. Rahaman, L.C. Zhang, M. Liu, W.D. Liu, Surface roughness effect on the friction and wear of bulk metallic glasses, Wear 332-333 (2015) 1231–1237.
H.I. Dawood, K.S. Mohammed, A. Rahmat, M.B. Uday, The inﬂuence of the surface roughness on the microstructures and mechanical properties of 6061 aluminium alloy using friction stir welding, Surf. Coat. Technol. 270 (2015) 272–283.